nilanjan/ce20100_lecture_9.pdf 1. is 269 33 grade ordinary portland cement 2. is 455 portland slag...
Post on 26-Mar-2020
Embed Size (px)
History Of Cement
The invention of Portland Cement is generally credited to Joseph Aspedin, an English Bricklayer in 1824. The Portland name was given because its color resembled the stone quarried on the Isle of Portland off the British coast.
In Germany and Belgium cement manufacturing started around 1855
In US manufacturing of cement started around 1870’s
Manufacturing of cement in India started in 1904 in Tamil Nadu but was fully established only by 1912. Till then for many years we were importing cement from England.
Cement – process of manufacture
TriCalcium Silicate 3CaO.SiO2 ~ C3S DiCalcium Silicate 2CaO.SiO2 ~ C2S TriCalcium Aluminate 3CaO.Al2O3 ~ C3A TetraCalcium Aluminoferrite 4CaO.Al2O3.Fe2O3 ~ C4AF
C3S + C2S constitute 65-75% by weight of cement and hydrate to form Ca(OH)2 (~25%) and Calcium Silicate hydrate (~50%) (also called tobermorite gel).
C3S ---- responsible for initial set and early strength C2S ---- increase in strength at ages beyond a week C3A ---- responsible for heat of hydration and also contributes slightly to early strength
Reducing C3A increases sulfate resistance C4AF --- reduces clinkering temp. Hydrates rapidly but contributes very less to strength
responsible for coloring effects.
Type I ---- normal Type II --- moderate sulfate resistant Type III – high early strength Type IV – low heat of hydration Type V --- high sulfate resistant Type I,II,III A --- air-entraining variety
Type I ---- general use; where special properties are not required Type II --- general use; moderate sulfate resistance and heat of hydration Type III – when high strength required. Has similarity chemically with Type I
but particles are ground finer. typical use cold or underwater structures Type IV – when low heat of hydration is required, typical use massive structures Type V --- when high sulfate resistance is required.
Air-entraining materials --- improved resistance to freeze-thaw; scaling caused by chemicals applied for snow/ice removal
White cement --- original color, grey comes in due to iron and manganese oxide, used for architectural purpose, curtain walls, tile grout and so on.
Types of Ordinary portland cement used in India (adopted from German Standards): grade 33, 43, 53
Fineness – greater cement fineness increases rate at which cement hydrates and accelerates strength development typically during the first week.
Soundness – ability of the hardened paste to retain volume after set. (free lime and magnesia responsible for lack of soundness). More sound less shrinkage.
Consistency – ability to flow. Depends on water-cement ratio. Setting time – affected by gypsum content, cement fineness, w/c ratio, admixtures Compressive strength – measured by 2 inch mortar cube. Compound composition and
fineness of cement affects it. Heat of hydration – heat generated when cement and water react. Increase in w/c ratio,
fineness of cement, curing temp increases heat of hydration. Specific gravity --- 3.15
Fineness measurement of cement (sq. cm per kg. of cement)
Blaine’s air permeability test Wagner’s turbidimeter
Conduction calorimeter – Heat of hydration
Materials to supplement cement
Contributes to the properties of hardened concrete through hydraulic or pozzolanic activity or both
Pozzolan :- Sliciceous or aluminosiliceous material that in finely divided form and presence of moisture, chemically reacts with calcium hydroxide released by hydration of portland cement to form calcium silicate hydrate and other cementitious material
Fly Ash Byproduct of combustion of pulverized coal in electric power generating plants During combustion, coal’s mineral impurities (clay, feldspar, quartz, shale) fuse in suspension and are carried away from combustion chamber by exhaust gas. The fused Materials cool and solidifies into spherical glassy particles.
Silica, alumina, iron, calcium 1.9-2.8
Granulated blast-furnace slag
Non-metallic hydraulic cement consisting essentially of silicates and aluminosilicates of calcium developed in a molten condition simultaneously with iron in blast-furnace. Molten slag rapidly chilled by quenching in water glassy sandlike granulated material
Silica Fume Byproduct obtained as a result of reduction of high purity quartz with coal in an electric-arc furnace in the manufacture of silicon or ferro-silicon alloy
Types Of Cement (commercially available)
Hydraulic Non -Hydraulic
Portland Cement Blends
Non-Portland hydraulic cements
Classification by BIS (Bureau Of Indian Standards)
Portland Cement Blends
Portland blast furnace cement
Portland fly ash cement
Portland pozzolan cement
Portland Silica Fume cement
Masonry Cement Non-Portland hydraulic cements
Super sulfated cements
Calcium sulfoaluminate cements
Portland Cement Grey
1. IS 269 33 Grade Ordinary Portland cement 2. IS 455 Portland Slag cement 3. IS 1489 Portland pozzolana cement - Part 1 Fly Ash based and Part 2
Calcined Clay based . 4. IS 3466 Masonry cement. 5. IS 6452 High alumina cement for structural use. 6. IS 6909 Super sulphated cement. 7. IS 8041 Rapid hardening Portland cement . 8. IS 8042 White Portland Cement. 9. IS 8043 Hydrophobic Portland Cement. 10.IS 8112 43 Grade Ordinary Portland cement. 11.IS 8229 Oil well cement 12.IS 12269 53 Grade Ordinary Portland cement 13.IS 12330 Sulphate resisting Portland cement 14.IS 12600 Low heat Portland Cement
According to BIS :
HYDRAULIC CEMENT :
• These cements are most commonly used nowadays.
• Hydraulic cements are materials which set and harden after combining with water, as a result of chemical reactions with the mixing water and, after hardening, retain strength and stability even under water.
NON HYDRAULIC CEMENT:
• Includes lime and gypsum plaster that must be kept dry in order to gain strength.
• Gain strength very slowly by absorption of carbon dioxide from the atmosphere to re-form calcium carbonate.
Portland cement is the most common type of cement as it is a basic ingredient of concrete, mortar and most non-specialty grout.
It is a fine, grey or white powder that is made by grinding Portland cement clinker, a limited amount of calcium sulfate which controls the set time, with other minor constituents
A hydraulic cement composed primarily of hydraulic calcium silicates
The most common use for Portland cement is in the production of concrete.
White Portland cement or white ordinary Portland cement (WOPC) is similar to ordinary, gray Portland cement in all respects except for its high degree of whiteness.
The color of white cement depends on raw materials and the manufacturing process. It is the metal oxides (primarily iron and manganese) that influence the whiteness and undertone of the material.
• White cements produce clean, bright colors, especially for light pastels. Many different colors can be created by adding pigments to concrete made with white cement.
Portland Cement Blends
PORTLAND BLAST FURNACE CEMENT Contains up to 70% ground granulated blast furnace slag, with the rest Portland clinker and a little gypsum. All compositions produce high ultimate strength. It is used as an economic alternative Portland sulfate-resisting and low-heat cements.
PORTLAND FLYASH CEMENT contains up to 30% fly ash so that ultimate strength is
maintained. Concrete water content, early strength this can be an economic alternative to ordinary Portland cement.
PORTLAND POZZOLAN CEMENT Includes fly ash cement also includes cements made from other natural or artificial pozzolans, since fly ash is a pozzolan, but also includes cements made from other natural or artificial pozzolans.
In countries where volcanic ashes are available (e.g. Italy, Chile, Mexico, the Philippines) these cements are often the most common form in use.
PORTLAND SILICA FUME CEMENT Addition of silica fume can yield exceptionally high strengths, and cements containing 5-20% silica fume are occasionally produced. contradictory shows no increases in the strength of cement paste, but substantial increases in concrete strength, when silica fume is used.
MASONRY CEMENTS Are used for preparing bricklaying mortars, and must not be used in concrete. They are usually complex proprietary formulations containing Portland clinker and a number of other ingredients that may include limestone, hydrated lime, air entertainers, retarders, water proofers and coloring agents.
NON PORTLAND HYDRAULIC CEMENTS
SLAG-LIME CEMENTS : Ground granulated blast furnace slag is not hydraulic on its own, but is “activated” by addition of alkalis, most economically using lime. They are similar to pozzolan lime cements in their properties.
CALCIUM ALUMINATE CEMENTS are hydraulic cements made primarily from limestone and bauxite. The active ingredients are monoca